MOLECULARLY IMPRINTED POLYMERS
Molecularly Imprinted Polymers for α-Tocopherol Delivery
1. Introduction 9
2. Materials and methods 12
2.1 Materials 12
2.2 HPLC analysis 12
2.3 Synthesis of α-tocopherol imprinted polymers 12
2.4 Binding experiments 13
2.5 Drug loading by the soaking procedure 13
2.6 In vitro release studies 13
3. Results and discussion 14
3.1 Synthesis of α-tocopherol imprinted polymers 14
3.2 Recognition properties of polymers 16
3.3 In vitro α-TP releasing properties 17
4. Conclusions 19
Imprinted Hydrophilic Nanospheres as Drug Delivery Systems for 5-Fluorouracil Sustained Release
1. Introduction 21
2. Materials and methods 23
2.1 Materials 23
2.3 Water content of spherical polymers 24
2.4 Binding experiments 25
2.5 Drug loading by the soaking procedure 25
2.6 In vitro release studies 26
2.7 HPLC analysis 26
2.8 Scanning electron microscopy 26
2.9 Dimensional analysis 26
3. Results and discussion 27
3.1 Synthesis of imprinted nanospheres 27
3.2 Evaluation of the imprinting effect: binding experiments in organic and in water media
3.3 In vitro release studies 31
4. Conclusions 33
Molecularly Imprinted Polymers for Selective Extraction and Sustained Release of Glycyrrhizic Acid
1. Introduction 35
2. Materials and methods 37
2.1 Materials 37
2.2 Synthesis of glycyrrhizic acid imprinted polymers 38
2.3 Binding experiments 39
2.4 Molecularly imprinted solid-phase extraction conditions 39
2.5 Extraction procedure 40 2.6 Molecularly imprinted solid-phase extraction of vegetable sample extracts 41
2.7 Drug loading by the soaking procedure 41
2.8 In vitro release studies 41
2.9 HPLC analysis 42
2.10 Analytical parameters 42
2.11 Statistical analysis 42
3. Results and discussion 43
3.2 Molecularly imprinted solid-phase extraction procedure and its optimisation
3.3 Molecularly imprinted solid-phase extraction of liquorice roots 48
3.4 Accuracy and precision 51
3.5 In vitro release studies 51
4. Conclusions 54
Surface Modifications of Molecularly Imprinted Polymers for Improved Template Recognition in Water Media
1. Introduction 57
2. Materials and methods 59
2.1 Materials 59
2.2 HPLC analyses 59
2.3 Synthesis of caffeine molecularly imprinted polymers 60
2.4 Epoxide rings opening 60
2.5 Phosphorilation procedure 62
2.6 Methylation procedure 62
2.7 Water absorption measurement 63
2.8 Binding experiments 63
2.9 Protein binding 64
2.10 Regeneration properties 64
3. Results and discussion 64
3.1 Synthesis of imprinted polymers 64
3.2 Surface modification 67
3.3 Hydrophilic properties of RAM-MIPs 68
3.4 Protein binding 70
3.5 Regeneration properties 71
New Restricted Access Materials combined to Molecularly
Imprinted Polymers for Selective Recognition/Release in Water Media
1. Introduction 73
2. Materials and methods 75
2.1 Materials 75
2.2 Instrumentation 76
2.3 Synthesis of p-acetaminophenol spherical molecularly imprinted polymers 77
2.4 Epoxide ring opening 78
2.5 Water content of spherical polymer 78
2.6 Binding experiments 79
2.7 Protein binding 79
2.8 Drug loading by soaking procedure 79
2.9 In vitro release studies 80
3. Results and discussion 80
3.1 Synthesis of imprinted polymers 80
3.2 Evaluation of the imprinting effect: binding experiments in organic media 82
3.3 Surface modification 83
3.4 Evaluation of the imprinting effect: binding experiments in water media 84
3.5 Water content of spherical polymers 84
3.6 Protein binding 85
3.7 In vitro release studies 86
Synthesis of a Novel Polymeric Materials with Biological Properties
1. Introduction 95
2. Materials and methods 97
2.1 Materials 97
2.2 Synthesis of the polymer containing ferulic acid (PMAA-FA) 98
2.3 Instrumentation 99
2.4 Evaluation of the antioxidant activity 100
2.4.1 Determination of scavenging effect on DPPH radicals 100
2.4.2 Linoleic acid emulsion system-thiocyanate assay 101 2.4.3 Evaluation of disposable phenolic groups by Folin-Ciocalteu procedure 102
2.4.4 Determination of total antioxidant activity 102 2.4.5 Evaluation of antioxidant activity on hydroxyl radical 103
2.5 Evaluation of the antifungal activity 103
3. Results and discussion 104
3.1 Synthesis of the polymer containing ferulic acid (PMAA-FA) 104
3.2 Characterisation of PMAA-FA 107
3.3 Evaluation of the antioxidant activity 108
3.3.1 Determination of scavenging effect on DPPH radicals 108 3.3.2 Linoleic acid emulsion system-thiocyanate assay 109 3.3.3 Evaluation of disposable phenolic groups by Folin-Ciocalteu procedure 110 3.3.4 Determination of total antioxidant activity 110 3.3.5 Evaluation of antioxidant activity on hydroxyl radical 110
3.4 Evaluation of the antifungal activity 111
3.5 UV protecting properties 112
Antioxidant and Spectroscopic Studies of Crosslinked Polymers containing Ferulic Acid
1. Introduction 115
2. Materials and methods 116
2.1 Materials 116
2.2 Instrumentation 116
2.3 Synthesis of bulk polymers 117
2.4 Synthesis of spherical polymers 118
2.5 Water content measurement 118
2.6 Evaluation of the antioxidant properties 119
2.6.1 Linoleic acid emulsion system-thiocyanate assay 119 2.6.2 Determination of scavenging activity on DPPH radicals 120 2.6.3 Determination of total antioxidant capacity 121 2.6.4 Determination of available phenolic groups in polymeric matrices 121
3. Results and discussion 122
3.1 Synthesis of antioxidant polymers 122
3.2 Polymers characterisation 124
3.2.1 FT-IR and NMR-MAS analyses 124
3.2.2 Physical characterisation 125
3.3 Evaluation of the antioxidant properties 127
3.3.1 Linoleic acid emulsion system-thiocyanate assay 127 3.3.2 Determination of scavenging activity on DPPH radicals 128 3.3.3 Determination of total antioxidant capacity 128
3.3.4 Determination of available phenolic groups in polymeric matrices 129
4. Conclusions 129
Covalent Insertion of Antioxidant Molecules on Chitosan and Gelatin by Free Radical Grafting Procedure
1. Introduction 131
2. Materials and methods 136
2.2 Instrumentation 136
2.3 Synthesis of chitosan conjugates 137 2.4 Synthesis of gelatin conjugates 138 2.5 Determination of scavenging effect on DPPH radicals 138
2.5.1 Scavenging properties of chitosan conjugates 138 2.5.2 Scavenging properties of gelatin conjugates 139
2.6 β-carotene-linoleic acid assay 140
2.7 Evaluation of disposable phenolic groups by Folin-Ciocalteu procedure 141
2.8 Determination of total antioxidant activity 141
2.8.1 Total antioxidant activity of chitosan conjugates 141 2.8.2 Total antioxidant activity of gelatin conjugates 142 2.9 Determination of scavenginge effect on hydroxyl radical (OH·) 143
3. Results and discussion 143
3.1 Synthesis of antioxidants conjugates 143
3.2 Characterisation of chitosan-antioxidant conjugates 147 3.3 Characterisation of gelatin-antioxidant conjugates 149 3.4 Determination of scavenging effect on DPPH radicals 154
3.5 β-carotene-linoleic acid assay 155
3.6 Evaluation of disposable phenolic groups by Folin-Ciocalteu procedure 156
3.7 Determination of total antioxidant activity 156
3.8 Hydroxyl radical (OH·) scavenging activity 157
Synthesis of Branched Polymers with Antifungal and Antioxidant Properties
1. Introduction 165
2. Materials and methods 167
2.1 Materials 167
2.2 Monomer synthesis 167
2.3 Synthesis of linear and branched polymers 169
2.4 Characterisation 171
2.4.1 Solubility tests 171
2.4.2 Elemental microanalyses 171
2.4.3 FT-IR spectroscopy 172
2.4.4 NMR spectroscopy 172
2.4.5 Dual detection size exclusion chromatography (DD-SEC) 172
3. Results and discussion 173
3.1 Monomer characterisation 173
3.2 Polymers characterization 175
3.2.1 Solubility tests 175
3.2.2 NMR spectroscopy 176
3.2.3 Evaluation of DD-SEC data 178
4. Conclusions and future work 186
In the last years, the development of novel polymeric systems has aroused a growing and considerable interest. Many researchers, indeed, have explored strategies to create polymeric materials that can grant new potential functions for applications in different fields, such as biomedical, pharmaceutical, cosmetic, food (packaging materials and coatings).
The aim of this PhD research project was the preparation of new functional polymers to be employed in these fields, exploring different synthetic strategies.
The PhD thesis is divided into three main sections.
The first one is focused on the synthesis of molecularly imprinted polymers (MIPs) and the evaluation of their applicability as Drug Delivery Systems (DDS) and stationary phases in Solid Phase Extraction (SPE). For this purpose, molecular imprinting technique was adopted to obtain polymeric materials with high selective recognition properties for a target molecule named template.
The second section reports on the synthesis and characterisation of polymeric antioxidants. This class of materials is characterised by higher stability and slower degradation rate than compounds with low molecular weight. To this aim, novel and simple approaches were developed involving the use of water soluble redox initiators or one-pot reaction in presence of 2,2’-azoisobutyronitrile (AIBN) to covalently bind an antioxidant molecule onto a polymeric chain.
The last section of this PhD work was carried out, during a six months
period, in the polymer research group at the Department of Pure and Applied Chemistry of University of Strathclyde. The aim of this study was the synthesis of branched polymers with biological activities via “Strathclyde route”. This facile, generic and cost effective route involves the conventional free radical polymerisation of vinyl monomers in the presence of chain transfer agents (CTAs) to inhibit cross-linking and gelation processes.
Molecularly Imprinted Polymers (MIPs) are synthetic materials characterised by recognition sites able to selectively rebind a target molecule in preference to other closely related compounds1.
MIPs are synthesised by polymerising functional and cross-linking monomers around a template molecule to obtain a highly cross-linked three-dimensional network polymer. The choice of the monomers depends on their ability to establish interactions with the functional groups of the template. Once polymerisation has taken place, the template is extracted to give a porous material containing binding sites that are complementary to the target molecule in terms of size, shape and functionalities (Figure 1.).
Figure 1. Schematic representation of the imprinting process.
The resulting MIPs are stable polymers with molecular recognition abilities and resistant to a wide range of conditions (pH, organic solvents, temperature, pressure).
6 The behaviour of imprinted polymers emulates the recognition and binding properties of natural biomolecules, such as antibodies and enzymes2.
MIPs, indeed, can mimic the interactions established by natural receptors to selectively retain a target molecule (i.e. antibody-antigen) but without the associated stability limitations. Furthermore, MIPs synthesis is relatively cheap and easy, making them a clear alternative to the use of natural receptors.
Three different approaches to prepare MIPs have been reported:
covalent, non-covalent and semi-covalent approaches. The covalent one3,
involves the formation of reversible covalent bonds between the template molecule and monomers before polymerisation. Then, the template is removed from the polymer structure by cleavage of the corresponding covalent bonds, which are re-formed upon rebinding of the analyte. The high stability of template-monomer interaction leads to a rather homogenous population of binding sites, minimising the existence of non-specific sites. However, the difficulty of designing an appropriate template-monomer complex in which covalent bond formation and cleavage are readily reversible under mild conditions makes this approach rather restrictive. An intermediate option is the semi-covalent approach4,5. In this case, the template is also covalently bound to a functional monomer, but the rebinding step is entirely non-covalent in nature. Finally, the non-covalent approach was introduced by Arshady and Mosbach6,
and is based on the formation of relatively weak non-covalent interactions (i.e. hydrogen bonding, ionic interactions) between template molecule and selected monomers before polymerisation. Today it represents the predominant method used, because it offers much more flexibility in terms of the functionalities on a template that can be targeted. The most obvious strength of this approach is that the experimental procedure is rather simple and it is generally assumed that a pre-polymerisation complex is formed between the template and functional
2 Mayes, A.G.; Whitcombe, M.J. Adv. Drug Del. Rev. 2005, 57, 1742. 3 Wulff, G.; Sarchan, A.A. Angew. Chem. Int. Ed. Engl. 1972, 11, 341. 4 Sellergren, B.; Andersson, L.I. J. Org. Chem. 1990, 55, 3381.
5 Withcombe, M.J.; Rodriguez, M.E.; Villar, P.; Vulfson, E. J. Am. Chem. Soc. 1995, 117, 7105.
7 monomers, which is then incorporated into the growing polymer network. The other great strength is the available wide range of functional monomers able to interact with almost any kind of template. However, there are some significant drawbacks derived from the fact that the template-monomer interactions are governed by an equilibrium process. Thus, in order to displace the equilibrium towards the formation of the template-monomer complex, a high amount of monomer is used. Consequently, the excess of free monomers is randomly incorporated to the polymeric matrix leading to the formation of non-selective binding sites which are indesiderable for most practical applications
MIPs were used for several different applications, such as chromatographic stationary phases7, enantiomeric separation8, solid-phase
extraction (SPE)9, and catalysis10; MIPs were also used as receptors11,
antibodies12, enzyme mimics13, and affinity and sensing materials14. In addition,
in recent years, MIPs have been reported to be suitable as drug delivery systems (DDS)15, and as base excipients for controlled release devices of several drugs16.
7 Hishiya, T.; Asanuma, H.; Komiyama, M. Polym. J. 2003, 35, 440. 8 Adbo, K.; Nicholls, I.A. Anal. Chim. Acta 2001, 435, 115.
9 Puoci, F.; Curcio, M.; Cirillo, G.; Iemma, F.; Spizzirri, U.G.; Picci, N. Food Chemistry 2008, 106, 836.
10 Anderson, C.D.; Shea, K.J.; Rychnovsky, S.D. Org. Lett. 2005, 7, 4879. 11 Haupt, K. Chem. Commun. 2003, 2, 171.
12 Svitel, J.; Surungiu, I.; Dzgoev, A.; Ramanathan, K.; Danielsson, B. J. Mater. Sci.-Mater. M. 2001, 12, 1075.
13 Nicholls, I.A.; Matsui, J.; Krook, M.; Mosbach, K. J. Mol. Recognit. 1996, 9, 652. 14 Syu, M.J.; Chiu, T.C.; Lai, C.Y.; Chang, Y.L. Biosens. Bioeletron. 2006, 22, 550. 15 Puoci, F.; Iemma, F.; Cirillo, G.; Picci, N.; Matricardi, P.; Alhaique, F. Molecules 2007, 12, 805.
Molecularly Imprinted Polymers for α-Tocopherol Delivery
In the last decade, many epidemiological, biological and clinical studies have proven that free-radical-induced oxidative damage to cell membranes, DNA, and proteins might play a causative role in several degenerative diseases, such as cancer, atherosclerosis, and other chronic diseases1,2,3,4,5. Reactive
oxygen and nitrogen species (ROS/RNS) are essential to energy supply, detoxification, chemical signalling, and immune function6. These species are
continuously produced in the human body, and their concentrations are controlled by endogenous enzymes (superoxide dismutase, glutathione peroxidase, and catalase). When there is an over-production of ROS and RNS, an exposure to external oxidant substances, or a failure in the defence
mechanisms, biomolecular damage may occur7. Some compounds, such as
α-tocopherol8, L-ascorbic acid9, and β-carotene10, generally named antioxidants,
might have beneficial effects in protecting human tissue against such damage.
1 Barnham, K.J.; Masters, C.L.; Bush, A.I. Nature Rev. Drug Discov. 2004, 3, 205. 2 Cooke, M.S.; Evans, M.D.; Dizdaroglu, M.; Lunec, J. FASEB J. 2003, 17, 1195. 3 Finkel, T.; Holbrook, N.J. Nature 2000, 408, 239.
4 Fernandez-Robredo, P.; Moya, D.; Rodriguez, J.A.; Garcia-Layana, A. IOVS 2005, 46, 1140.
5 Tian, N.; Thrasher, K.D.; Gundy, P.D.; Hughson, M.D.; Manning Jr, R.D. Hypertension 2005, 45, 934.
6 Young, I.S.; Woodside, J.V. J. Clin. Pathol. 2001, 53, 176.
7 Iemma, F.; Cirillo, G.; Puoci, F.; Trombino, S.; Castiglione, M.; Picci, N. J. Pharm. Pharmacol. 2007, 59, 597.
8 Kalogeropouloset, N.; Chiou, A.; Mylona, A.; Ioannou, M.S.; Andrikopoulos, N.K. Food Chem. 2007, 100, 509.
9 Jayathilakan, K.; Sharma, G.K.; Radhakrishna, K.;Bawa, A.S. Food Chem. 2007, 100, 662.
10 Bairati, I.; Meyer, F.; Jobin, E.; Gelinas, M.; Fortin, A.; Nabid, A.; Brochet, F.; Tetù, B. Int. J. Cancer 2006, 119, 2221.
10 Our interest focused on α-tocopherol (α-TP, Figure 1.1), a representative oil-soluble antioxidant of the vitamin E type11. The physiological relevance of
α-TP, and the severe pathological consequences of its deficiency, impose a major challenge to the living organisms for sustaining an adequate supply of this compound to different tissues, particularly those highly sensitive to α-TP deficiency such as the brain and gonads12. α-TP deficiency could be overcome
by dietary supplementation, and several studies have described the beneficial effect of oral supplementation with vitamin E on the prevention and treatment of cardiovascular diseases and cancer13.
The goal of this work is the preparation of a new controlled drug delivery device for α-TP oral supplementation14.
A controlled drug delivery system maximises the drug efficacy and safety and provides a suitable rate of delivery of the therapeutic dose, at the most appropriate site in the body. This would prolong the duration of the drug activity, to reduce side-effects, and minimise administration frequency, thus enhancing patient compliance15,16.
Our approach for the realisation of α-TP delivery system is based on molecularly imprinted technology and the non-covalent approach was employed17. This method involves the pre-organisation of functional monomers
around a template molecule to form a pre-polymerisation complex by hydrogen bonding, ionic, or hydrophobic interactions. The formed complex is subsequently radically copolymerised in a solution containing a high ratio of a suitable cross-linker to form, after the subsequent removal of the template, macroporous matrices having microcavities that retain specific orientation of
11 Qian, J.; Morley, S.; Wilson, K.; Nava, P.; Atkinson, J.; Manor, D. J. Lipid Res. 2005, 46, 2072.
12 Mardones, P.; Rigotti, A. J. Nutr. Biochem. 2004, 15, 252.
13 Morris, M.C.; Evans, D.A.; Tangney, C.C.; Bieinias, J.L.; Wilson, R.S.; Aggarwal, N.T.; Scherr, P.A. Am. J. Clin. Nutr. 2005, 81, 508.
14 Puoci, F.; Cirillo, G.; Curcio, M.; Iemma, F.; Parisi, O.I.; Castiglione, M.; Picci, N. Drug Deliv. 2008, 15, 253.
15 Cunliffe, D.; Kirby, A.; Alexander, C. Adv. Drug Del. Rev. 2005, 57, 1836. 16 Alvarez-Lorenzo, C.; Concheiro, A. J. Chromatogr. 2004, 804, 231.
17 Caro, E.; Marce, R.M.; Cormack, P.A.G.; Sherrington, D.C.; Borrull, F. Anal. Chim. Acta 2006, 562, 145.
11 functional groups in a three-dimensional structure complementary to that of the template about which they were formed18.
The aim of this study was the preparation of molecularly imprinted polymers able to selectively rebind and release α-TP in gastrointestinal simulating fluids. MIPs were synthesised using methacrylic acid (MAA) as functional monomer and ethylene glycol dimethacrylate (EGDMA) as cross-linking agent19. The recognition properties of the synthesised materials were tested both in organic (i.e., acetonitrile) and in aqueous media (i.e., an ethanol/water 6/4, v/v mixture). Considerable differences in the recognition characteristics between imprinted and non-imprinted polymers have been observed. The selectivity of the polymeric device was also evaluated using a molecule structurally similar to the template, in particular 6-hydroxy-2,5,7,8-tetramethylchroman-2-carboxylic acid (HMCA) was employed (Figure 1.1). Finally the release profile of α-TP in gastrointestinal simulating fluids was evaluated.
Figure 1.1 Chemical structures of α-tocopherol (α-TP) and
6-hydroxy-2,5,7,8-tetramethylchroman-2-carboxylic acid (HMCA).
18 Caro, E.; Marce, R.M.; Cormack, P.A.G.; Sherrington, D.C.; Borrull, F. J. Sep. Sci. 2006, 29, 1230.
19 Puoci, F.; Cirillo, G.; Curcio, M.; Iemma, F.; Spizzirri, U.G.; Picci, N. Anal. Chim. Acta 2007, 593, 164.
2. Materials and methods
Ethylene glycol dimethacrylate (EGDMA), methacrylic acid (MAA), 2,2’-azoisobutyronitrile (AIBN), α-tocopherol (α-TP), and 6-hydroxy-2,5,7,8-tetramethylchroman-2-carboxylic acid (HMCA) were obtained from Sigma Chemical Co. (St. Louis, MO).
All solvents were reagent grade or HPLC-grade, they were used without further purification, and they were provided by Fluka Chemie (Buchs, Switzerland).
2.2 HPLC analysis
The liquid chromatography consisted of a Jasco BIP-I pump and a Jasco
UVDEC-100-V detector set at 292 nm. A 250×4 mm C-18 Hibar® column,
particle size 10 μm (Merck, Darmstadt, Germany) was used. The mobile phase was methanol and the flow rate was 1.0 mL/min.
2.3 Synthesis of α-tocopherol imprinted polymers
α-TP imprinted polymers (MIPs) were prepared using MAA as functional monomer. Briefly, 0.43 g (1 mmol) of template α- tocopherol and 1.38 g (16 mmol) of MAA were dissolved in 5.25 mL of chloroform in a thick walled glass tube, and then 4.95 g (25 mmol) of EGDMA and 0.100 g (0.60 mmol) of AIBN were added. The tube was purged with nitrogen, sonicated for 10 min, and then photo-polymerised for 24 h with 360 nm light at 4°C. After the photolysis, the tubes were incubated at 60°C for 24 h. The resultant bulk rigid polymers were crushed, ground into powder, and strained through a 63 nm stainless steel sieve. The sieved MIP materials were collected and the very fine powder, suspended in the supernatant solution (acetone), was discarded. The resultant MIPs were placed in a Soxhlet and extracted with 200 mL of a tetrahydrofuran:acetic acid (8:2 v/v) mixture for at least 48 h, followed by 200 mL of tetrahydrofuran for others 48 h and then they were dried in an oven at 60°C overnight. The washed MIP materials were checked to be free of
α-13 tocopherol and any other compound by high-performance liquid chromatography (HPLC).
Non-imprinted polymers (NIPs), to act as a control, were also prepared when polymerisation was carried out in the absence of α-tocopherol.
2.4 Binding experiments
The binding efficiency of polymeric matrices toward α-TP was evaluated in the rebinding experiments, which were performed both in acetonitrile and in an ethanol:water mixture (6:4 v/v). Briefly, 50 mg of polymer particles were mixed with 1 mL of an α-TP solution (0.2 mM) in a 1 mL eppendorf and sealed. The eppendorf tubes were oscillated by a wrist action shaker (Burrell Scientific) in a water bath at 37 ± 0.5°C for 24 h. Then the mixture was centrifuged for 10 min (10000 rpm) in an ALC® microcentrifugette®
4214 and the α-TP concentration in the liquid phase was measured by HPLC. The amount of α-TP bound to the polymer was obtained by comparing its concentration in the MIPs samples to the NIPs samples.
The same experiments were performed using HMCA solutions.
Experiments were repeated five times, and results were expressed as means (± SD).
2.5 Drug loading by the soaking procedure
Two grams of polymeric matrix were immersed in 20 mL of an α-TP solution (5.5 mM) in acetonitrile and soaked for 3 days at room temperature. During this time, the mixture was continuously stirred, and then the solvent was removed. Finally, the powder was dried under vacuum overnight at 40°C.
2.6 In vitro release studies
Release studies were done using the dissolution method described in the USP XXIV (apparatus 1-basket stirring element). To mimic the pH of the digestive tract, 0.1 N HCl (pH 1.0) was used as simulated gastric fluid, and after 2 h, disodium hydrogen phosphate (0.4 M) was added to adjust the pH value to
14 6.8 to simulate the intestinal fluid. To improve the solubility of released α-TP in the simulated fluid, each testing sample contained 0.1% of sodium dodecylsulfate (SDS).
The experiments were performed as follows: 30 mg of MIP and NIP particles loaded with α-TP were dispersed in flasks containing 10 mL of 0.1 N HCl and maintained at 37 ± 0.5°C in a water bath for 2 h under magnetic stirring (50 rpm). Disodium hydrogen phosphate (0.4 M, 5 mL) was then added to the samples. These conditions were maintained throughout the experiment. To characterise the drug release, 2 mL of samples were drawn from the dissolution medium at designated time intervals, and the same volume of simulated fluid was supplemented. α-TP was determined by HPLC analysis, and the amount of α-TP released from five samples of each formulation was used to characterise the drug release.
The percentage of released TP was calculated considering 100% the α-TP content in polymeric samples after drying procedure20.
Experiments were repeated five times and were expressed as means (± SD).
3. Results and discussion
3.1 Synthesis of α-tocopherol imprinted polymers
For the preparation of molecularly imprinted polymers, generally three different approaches have been developed: the covalent, the semi-covalent, and the non-covalent approach.
The first one, pioneered by Wulff’s group21, involves the formation of a
complex between functional monomers and template molecules via reversible covalent bond (such as boronate ester, ketal and acetal, or Schiff base) both prior to polymerisation and in the rebinding experiments.
20 Pitarresi, G.; Pierro, G.; Giammona, G.; Iemma, F.; Muzzalupo, R.; Picci, N. Biomaterials 2004, 25, 4333.
15 In the semi-covalent approach, covalent interactions are involved in MIP synthesis, while the subsequent rebinding phase is based on non-covalent interactions.
The non-covalent approach, pioneered and extensively developed by Mosbach and coworkers22, instead, involves only non covalent interactions (such as hydrogen bonds, ionic interactions, hydrophobic interactions, and metalion chelating interactions) for both the molecular imprinting process and the subsequent rebinding. This approach is the most flexible because of the absence of complicated synthetic processes and the subsequent possibility of using a far greater variety of functional monomers.
For these reasons, we chose the non-covalent imprinting method for the preparation of bulk imprinted polymers for the sustained/controlled release of α-tocopherol. MAA was used as functional monomer and EGDMA as cross-linker.
The whole of the reaction conditions have to maximise the interactions between the template and the functional monomer and consequently to ensure strong and selective binding of the substrate to the polymeric matrices. Two main parameters must be considered. The first is the polymerisation temperature. The formation of the complex is a dynamic process and, when a template with few functional groups able to create hydrogen bonds is used, a low temperature is needed to reduce the kinetic energy of the system. In this case, indeed, a high temperature could drive the equilibrium away from the template-functional monomer complex toward the unassociated species, resulting in a decrease in the number of imprinted cavities and thus in the recognition properties of the final materials. Better results were obtained using photopolymerisation processes. Furthermore, in these conditions, a lesser degree of polymerisation was observed, so the performance of photopolymerised materials must be improved after high-temperature treatment of the initially formed polymer23. Based on
22 Zhang, H.; Ye, L.; Mosbach, K. J. Mol. Recognit. 2006, 19, 248.
23 Cheong, S.H.; McNiven, S.; Rachkov, A.; Levi, R.; Yano, K.; Karube, I. Anal. Chem. 1997, 69, 2017.
16 these consideration, MIPs were synthesised under UV irradiation at 4°C for 24 h and then with thermal stabilization at 60°C for another 24 h.
The second parameter to be considered is the nature of the porogenic agent. The inert solvent used in the polymerisation mixture may play a major role in determining the properties (surface area, internal pore volume, etc.) of the resulting polymer. Moreover, since polar solvents are more able to solvate polar molecules, this leads to the disruption of H-bonds between the template and the functional monomer24,25. Thus, our general procedure, employed to improve the
recognition properties of molecularly imprinted polymers, was the choice of the least polar solvent in which the reagents were dissolved. In our case, we chose chloroform.
3.2 Recognition properties of polymers
Evaluation of the capacity of the matrices to recognise and bind the template was performed in acetonitrile (organic medium), and also in ethanol/water mixture (6/4 v/v).
Polymeric particles were incubated with an α-TP solution 0.2 mM for 24 hours. Table 1.1 shows the percentage of α-TP bound by imprinted and non-imprinted polymers.
It should be noted that the synthesised materials have good recognition properties. The imprinted polymers, indeed, bind much more template than do their respective non-imprinted counterparts, confirming the presence of α-TP specific cavities. The higher amounts of bound α-TP in aqueous medium, compared with that in acetonitrile, are ascribable to the presence of more hydrophobically driven bonds, the extent of which depends on the hydrophobicity of the template and the surface of the material. But also in this case, MIPs samples bind much more α-TP than NIPs ones.
24 Whitcombe, M.J.; Rodriguez, M.E.; Villar, P.; Vulfson, E.N. J. Am. Chem. Soc. 1995, 117, 7105.
25 Cheong, S.H:; McNiven, S.; Rachkov, A.; Levi, R.; Yano, K.; Karube, I. Macromolecules 1997, 30, 1317.
Table 1.1 Percentage of bound α-TP and HMCA by MIP and NIP in organic (CH3CN) and
aqueous (EtOH/H2O 6/4 v/v mixture) media.
Bound α-TP (%) Bound HMCA (%)
CH3CN EtOH/H2O CH3CN EtOH/H2O
MIP 27 ± 0.9 99 ± 0.7 9 ± 1.8 44 ± 0.6
NIP 1 ± 0.7 67 ± 1.2 14 ± 1.6 44 ± 1.1
Well imprinted polymers are asked to interact selectively with the template around which they are formed, compared with some structurally analogous molecules. The selectivity of the imprinted polymers was tested by performing the same binding experiments using 6-hydroxy-2,5,7,8-tetramethylchroman-2-carboxylic acid (HMCA) instead of α-TP (Table 1.1). The chemical difference between the two analytes drives the interactions with the polymeric matrices. The carboxylic group of HMCA makes this molecule much more hydrophilic than α-TP.
It should be noted that the polymers practically do not interact with HMCA in organic media, whereas in water solution the binding percentage of the analog is higher but considerably lower than that of the original template. Furthermore, in all the environments tested, the amounts of HMCA bound by the imprinted and the non-imprinted polymers are practically the same, and this clearly shows the non-specific nature of these interactions.
3.3 In vitro α-TP releasing properties
The possibility of employing the synthesised MIPs as devices for the controlled release of α-TP in gastrointestinal simulated fluids was investigated. In vitro release studies were performed by immersing aliquots of the microparticles loaded with α-TP at pH 1.0 (simulated gastric fluid) for 2 hours and then at pH 6.8 (simulated intestinal fluid) using the pH change method. To
18 improve the solubility of α-TP in aqueous media, SDS was added to the solutions.
Our hypothesis was that α-TP imprinted polymers have a better ability to control the drug release in compared with non-imprinted polymers due to the presence of specific binding sites in the polymeric network that are able to release the drug much more slowly. The experimental data confirm this hypothesis; the drug release from NIPs was indeed remarkably faster than that observed from MIPs. In particular, while in the first case the drug is completely released within 4 hours, only 50% of α-TP was released from MIP samples during the same period (Figure 1.2).
Figure 1.2 Release profile of α-TP from MIPs and NIPs
in gastrointestinal simulating fluids.
After the pH changing, in intestinal simulating fluids, α-TP release from MIPs continues, and in 24 hours the percentage of α- TP released was about 80% (100% within 40 h). These remarkable differences depend on the different recognition properties of the two polymeric matrices. The non-imprinted polymers, indeed, do not have specific binding cavities for the drug, while the MIP samples, because of their specific structure, strongly bound α-TP by
non-0 20 40 60 80 100 0 5 10 15 20 25 30 Time (h) Re le as e ( % ) NIPs MIPs
19 covalent interactions in the cavities formed during the polymerisation procedure in the presence of the analyte.
This observation supports a model of retention mechanism, which assumes that the acid groups of the selective sites have stronger interaction with the drug than the non-selective sites. At low pH (1.0) values, the carboxylic groups are not ionised and there is a good interaction with the template. These results might help us to understand the behavior of these matrices when the pH increases. Under these conditions, that simulate the intestinal fluid, in the non-imprinted polymers the antioxidant is bound with non-covalent interactions on the surface of the matrices. At pH 6.8, the diffusion rate of the buffer on the polymer surface is fast, the carboxylic groups are ionised, and the drug is rapidly released. Instead, in the MIP case, the diffusion rate of the buffer into specific cavities of imprinted polymers is slower, and the functional groups are ionised more slowly, resulted in well controlled release.
For these reasons, the rate of the release was considerably different, and MIPs represent a very useful polymeric device for the selective and controlled release of the antioxidant agent in gastrointestinal fluids.
The aim of this work was the preparation of a specific oral delivery system for α-TP. To this end, we used molecular imprinting tecnique.
The polymerisation conditions involve the use of MAA and EGDMA as functional monomer and crosslinking agent, respectively. To improve the recognition properties of the synthesised materials, a photopolymerisation procedure was employed. Before evaluating of the α-TP release profile, the recognition and selectivity properties of the polymeric devices, both in organic and in aqueous media, were studied performing rebinding experiments. The percentage of α-TP bounded by the molecularly imprinted polymers was remarkably higher in both the environments tested compared with the non-imprinted ones, and MIPs also showed a high selectivity.
20 In vitro release tests were performed in gastrointestinal simulating fluids. MIPs samples was found to be able to release slowly the drug compared with NIPs, thus the synthesised polymeric matrices represent a very useful novel controlled drug dosage device.
Imprinted Hydrophilic Nanospheres as Drug Delivery Systems for
5-Fluorouracil Sustained Release
5-Fluorouracil (5-FU; Figure 2.1) is a widely used antineoplastic agent for the treatment of many types of cancers, such as colorectal, breast, head and neck malignancies1. Its endurance and longevity in cancer chemoterapy is due to
the fact that 5-FU is the only anticancer agent on the market that shows synergism with the most other anticancer drugs in combination therapy2.
Figure 2.1 Chemical structures of 5-fluorouracil (5-FU) and uracil (U).
On the other hand, it is effective against cancers refractory to other treatments. Despite these advantages, the use of 5-FU is limited by its quick metabolism in the body, therefore the maintenance of high serum concentrations of this drug to improve its therapeutic activity is needed. The maintenance of these serum concentrations requires continuous administrations, but 5-FU shows
1 Di Paolo, A.; Romano, D.; Vannozzi, F.; Falcone, A.; Mini, E.; Cionini, L.; Ibrahim, T.; Amadori, D.; Del Tacca, M. Clin. Pharmacol. Ther. 2002, 72, 627.
2 Al Safarjalani, O.N.; Rais, R.; Shi, J.; Schinazi, R.F.; Naguib, F.N.M.; El Kouni, M.H. Cancer Chemother. Pharmacol. 2006, 58, 692.
22 severe toxic effects; consequently reaching and/or exceeding the toxic concentration must be avoided3.
In order to improve therapeutic index and reduce toxic effects of this drug, numerous studies in literature are aimed at design of devices for the controlled release of 5-FU, many of them are based on polypeptidic and polysaccharidic systems4.
In our previous study5, irregular and not swellable microparticles of 5-FU imprinted polymers by employed bulk polymerisation were prepared, and their application as devices for controlled release of this drug was demonstrated. In order to obtain a better control on particle size and shape, and so also on the 5-FU release profile, in this work molecularly imprinted hydrogel nanospheres have been synthesised applying straightforward method such as precipitation polymerisation6.
Coupling the properties of hydrogels, nanospheres and MIPs it is possible to obtain very useful systems to be applied in drug delivery field.
Firstly, due to their significant water content, hydrogels possess a degree of flexibility very similar to natural tissue, which minimises potential irritation to surrounding membranes and tissues7. Moreover, the high swelling properties of these materials improved their recognition characteristics, because of the enhanced accessibility of template to the imprinted cavities.
Molecularly imprinted polymers (MIPs) are tailor-made materials with high selectivity for the template molecule8,9 and, as reported in literature10, these
3 Johnson, K.R.; Young, K.K.; Fan, W. Clin. Cancer Re. 1999, 5, 2559.
4 Fournier, E.; Passirani, C.; Colin, N.; Breton, P.; Sagodira, S.; Benoit, J.P. Eur. J. Pharm. Biopharm. 2004, 57, 189.
5 Puoci, F.; Iemma, F.; Cirillo, G.; Picci, N.; Matricardi, P.; Alhaique, F. Molecules 2007, 12, 805.
6 Cirillo, G.; Iemma, F.; Puoci, F.; Parisi, O.I.; Curcio, M.; Spizzirri, U.G.; Picci, N. J. Drug Target. 2009, 17, 72.
7 Byrne, M.E.; Park, K.; Peppas, N.A. Adv. Drug Deliv. Rev. 2002, 54, 149.
8 Puoci, F.; Curcio, M.; Cirillo, G.; Iemma, F.; Spizzirri, U.G.; Picci, N. Food Chem. 2008, 106, 836.
9 Beltran, A.; Caro, E.; Marcé, R.M.; Cormack, P.A.G.; Sherrington, D.C.; Borrull, F. Anal. Chim. Acta 2007, 597, 6.
23 synthetic molecularly selective receptors have broad application in many areas of science and the area of greatest potential, and probably an area of greatest challenge, is that of therapeutics and medical therapy. They have been applied usefully as excipients to modify drug release from solid dosage forms.
Finally, advances in nanobiotechnology have resulted in the evolution of several novel colloidal carriers such as liposomes, polymeric micelles nanoparticles, and nanoemulsions to maximise tumor cell killing effect during the tumor growth phase, and to protect the surrounding healthy cells from unwanted exposure to the excess cytotoxic agent11. Polymeric nanoparticles are
the most attractive colloidal carriers owing several merits such as ease of purification and sterilisation, drug targeting possibility, and sustained release action12.
In conclusion, the delivery of an anticancer drug by molecularly imprinted nanospherical hydrogels offers the possibility of maximising its efficacy and safety and providing a suitable rate of delivery of the therapeutic dose at the most appropriate site in the body, in order to prolong the duration of the pharmacological activity, to reduce the side effects and to minimise the administration frequency, and thus enhancing patient compliance13.
The purpose of this study was to investigate the possibility of employing these monodispersed imprinted nanoparticles as devices for the controlled/sustained release of 5-FU in biological fluids.
2. Materials and methods
Ethylene glycol dimethacrylate (EGDMA), methacrylic acid (MAA), 2,2’-azoisobutyronitrile (AIBN), 5-fluorouracil (5-FU) and uracil (U) were obtained from Sigma-Aldrich (Sigma Chemical Co., St. Louis, MO).
11 Yadav, A.K.; Mishra, P.; Jain, S.; Mishra, P.; Mishra, A.K.; Agrawal, G.P. J. Drug Target 2008, 16, 464.
12 Allemann, E.; Gurny, R.; Doelker, E. Eur. J. Pharm. Biopharm. 1993, 39, 173. 13 Hilt, J.Z.; Byrne, M.E. Adv. Drug Deliv. Rev. 2004, 56, 1599.
24 All solvents were reagent grade or HPLC-grade and used without further purification and they were provided by Fluka Chemika-Biochemika (Buchs, Switzerland).
2.2 Synthesis of 5-FU spherical molecularly imprinted polymers
Spherical molecularly imprinted polymers (SMIP) were prepared by precipitation polymerisation using 5-fluorouracil as template, MAA as functional monomer and ethylene glycol dimethacrylate as crosslinking agent.
General synthetic procedure was reported: template (1 mmol) and MAA (8 mmol) were dissolved in a mixture of acetonitrile (20 mL) and methanol (20 mL), in a 100 mL round bottom flask and then EGDMA (10 mmol) and AIBN (50 mg) were added. The polymerisation mixture was degassed in a sonicating water bath, purged with nitrogen for 10 min cooling with an ice-bath. The flask was then gently agitated (40 rpm) in an oil bath. The temperature was increased from room temperature to 60°C within 2 h, and then kept at 60 °C for 24 h. At the end of the reaction, the particles were filtered, washed with 100 mL of ethanol, 100 mL of acetone and then with 100 mL of diethyl ether. The template was extracted by ‘‘Soxhlet apparatus’’ using methanol:acetic acid mixture (1:1 v/v, 100mL) for at least 48 h, followed by methanol for another 48 h, and monitoring the drug concentration in the extraction solvent by HPLC. Particles were successively dried under vacuum overnight at 40 °C.
Spherical non-imprinted polymers (SNIP), that act as a control, were also prepared when polymerisation was carried out in the absence of 5-fluorouracil.
2.3 Water content of spherical polymers
Aliquots (40-50 mg) of the nanospheres dried to constant weight were placed in a tared 5-mL sintered glass filter (Ø10 mm; porosity, G3), weighted, and left to swell by immersing the filter plus support in a beaker containing the swelling media: phosphate buffer (pH 7.4, simulated biological fluids). At predetermined times (2 - 4 - 8 -10 - 15 - 20 - 24 h), the excess water was
25 removed by percolation at atmospheric pressure. Then, the filter was placed in a properly sized centrifuge test tube by fixing it with the help of a bored silicone stopper, then centrifuged at 3500 rpm for 15 min and weighted. The filter tare was determined after centrifugation with only water. The weights recorded at the different times were averaged and used to give the water content percent (WR %) by the following equation (1) :
×d d s
where Ws and Wd are weights of swollen and dried spherical microparticles,
Each experiment was carried out in triplicate.
2.4 Binding experiments
Binding experiments were performed both in organic (acetonitrile) and in aqueous media (phosphate buffer pH 7.4).
Briefly, 50 mg of polymer particles were mixed with 5 mL of a 5-FU solution (0.3 mM) in a 10 mL conical centrifugation tube and sealed. The tubes were oscillated by a wrist action shaker (Burrell Scientific) in a water bath for 24 h. Then the mixture was centrifuged for 10 min (10000 rpm) and the 5-FU concentration in the liquid phase was measured by HPLC. The amount of 5-FU bound to the polymer was obtained by comparing its concentration in the imprinted samples to the non-imprinted ones.
The same experiments were performed using uracil solution. Experiments were repeated five times.
2.5 Drug loading by the soaking procedure
Polymeric matrix (2.0 g) was immersed in a 5-FU solution in acetonitrile (20 mL, 5.5 mM) and soaked for 3 days at room temperature. During this time, the mixture was continuously stirred and then the solvent was removed by filtration. Finally the powder was dried under vacuum overnight at 40°C.
26 2.6 In vitro release studies
Release studies were carried out using the dissolution method described in the USP XXIV (apparatus 1-basket stirring element).
The samples were dispersed in flasks containing 10 mM phosphate buffer solution (pH 7.4 simulating biological fluids, 10 mL). Thus samples were drawn from dissolution medium at appropriate time intervals to determine the amounts of released drug by HPLC. The amount of 5-fluorouracil released from six samples of each formulation was used to characterise the drug release.
The same experiments were performed using particles loaded with uracil.
Experiments were repeated five times.
2.7 HPLC analysis
A Jasco BIP-I pump and a Jasco UVDEC-100-V detector set at 266 nm14
was used. A 250 × 4 mm C-18 Hibar® column, 10 μm particle size (Merck,
Darmstadt, Germany) was employed. The mobile phase was methanol/phosphate buffer 5 mM, pH 6.8 (9/1, v/v) and the flow rate was 0.5 mL/min.
2.8 Scanning electron microscopy
Scanning electron microscopy (SEM) photographs were obtained with a Jeol JSMT 300 A; the surface of the samples was made conductive by deposition of a gold layer on the samples in a vacuum chamber.
2.9 Dimensional analysis
Approximate range in particle size was determined by measuring 300 particles per each sample with the use of an image processing and analysis system, a Leica DMRB equipped with a LEICAWild 3D stereomicroscope.
14 Fournier, E.; Passirani, C.; Colin, N.; Breton, P.; Sagodira, S.; Benoit, J.P. Eur. J. Pharm. Biopharm. 2004, 57, 189.
3. Results and discussion
3.1 Synthesis of imprinted nanospheres
5-Fluoruracil molecularly imprinted polymers were synthesised
employing the non-covalent approach15, in which the interactions between
template molecule and polymeric matrices were based on H-bonds, the dominant interactions in biological systems. Furthermore, this approach is more convenient because of the easy access to a broad range of functional monomers from commercial sources.
Conventionally, MIPs are synthesised by bulk polymerisation methods in a porogenic solvent and block co-polymer particles with the desired size are obtained by grinding and sieving16,17. However, this method yields particles with
limited control on particle size and shape.
In literature, several attempts have been applied to produce monodisperse molecularly imprinted polymeric particles using methods such as suspension polymerisation in water18, dispersion polymerisation19, liquid
perfluorocarbon20, and via aqueous two-step swelling polymerisation21.
However, during the polymerisation procedure, these techniques require water or highly polar organic solvents, which frequently decrease specific interactions between functional monomers and template molecules. Precipitation technique not only allows to avoid these disadvantages, but also to obtain monodispersed molecularly imprinted micro- and nanospheres, without the integrity and stability of recognition sites are compromised22. Moreover, spherical shape
15 Puoci, F.; Cirillo, G.; Curcio, M.; Iemma, F.; Spizzirri, U.G.; Picci, N. Anal. Chim. Acta 2007, 593, 164.
16 Caro, E.; Marcé, R.M.; Borrull, F.; Cormack, P.A.G.; Sherrington, D.C. Trends Anal. Chem. 2006, 25, 143.
17 Puoci, F.; Cirillo, G.; Curcio, M.; Iemma, F.; Parisi, O.I.; Castiglione, M.; Picci, N. Drug Deliv. 2008, 15, 253.
18 Lai, J.P.; Lu, X.Y.; Lu, C.Y.; Ju, H.F.; He, X.W. Anal. Chim. Acta 2001, 442, 05. 19 Say, R.; Birlik, E.; Ersoz, A.; Yilmaz, F.; Gedikbey, T.; Denizli, A. Anal. Chim. Acta 2003, 480, 251.
20 Mayes, A.G.; Mosbach, K. anal. Chem. 1996, 68, 769.
21 Piscopo, L.; Prandi, C.; Coppa, M.; Sparnacci, K.; Laus, M.; Lagana, A.; Curini, R.; D’Ascenzo, G. Macromol. Chem. Phys. 2002, 203, 532.
28 should be advisable in order to avoid swelling anisotropic behaviour associated with other geometries23.
In our protocol, MAA as functional monomer and EGDMA as crosslinking agent were used.
Spherical geometry and the practically monodispersion of prepared samples were confirmed by Scanning Electron Micrographs (Figure 2.2) and dimensional analysis. Polymerisation feeds composition and mean particle sizes (dn) of the microspheres are shown in Table 2.1.
Figure 2.2 Scanning electron micrograph of SMIP.
Table 2.1 Polymerisation feed composition and mean particle sizes (dn) of nanospheres
as means ± SD. POLYMER 5-FU/MAA/EGDMA (mmol) dn (nm) POLYDISPERSIVITY SMIP 1.0 / 8.0 / 10.0 274 1.03 SNIP -- / 8.0 /10.0 268 1.01
23 Puoci, F.; Iemma, F.; Spizzirri, U.G.; Cirillo, G.; Castiglione, M.; Picci, N. Macromol. Ind. J. 2007, 3, 64.
29 3.2 Evaluation of the imprinting effect: binding experiments in organic and in water media
The imprinting effect of synthesised materials was evaluated by binding experiments in which amounts of polymeric particles were incubated with a 5-FU solution (0.3 mM) for 24 hours. These experiments were performed in organic (acetonitrile) and in water (buffered water solution at pH = 7.4) media.
As shown in Table 2.2, in both binding media, imprinted nanosphers were able to bind much more template than the respective non-imprinted ones, confirming the presence of imprinted cavities in their structure.
Table 2.2 Percentages of bound 5-FU and U and water content (%) at pH 7.4.
Data are shown as means ± SD.
MATRIX % 5-FU bound % U bound Water content (%)
CH3CN pH 7.4 CH3CN pH 7.4 pH 7.4 SMIP 32± 1.1 36±1.6 14± 1.4 16± 1.6 377 ± 0.3 SNIP 7± 1.3 10± 1.9 11± 1.1 14± 1.8 380 ± 0.5
In literature, different approaches were applied to make a quantitative determination of the imprinting effect24. The imprinting efficiency α is the
easiest way to highlight the recognition properties in a MIP. In our work, α5-FU
was determined as the ratio between the amount (%) of 5-FU bound by SMIP and SNIP25; these values (4.6 in CH
3CN and 3.6 in water media) clearly prove
the specificity of the interaction between the template and the functional groups on the polymeric nanoparticles.
To evaluate cross-reactivity of imprinted polymers towards 5-fluorouracil analogue molecules, the same binding experiments were performed using uracil, that differs from 5-FU only in substituent at position 5 of the ring (Figure 2.1). As reported for 5-FU, αU was also determined as ratio between U
24 Ye, L.; Mosbach, K. Chem. Mater. 2008, 20, 859.
30 bound by SMIP and SNIP, respectively. The very low values (1.3 in CH3CN and
1.1 in water media) show the high chemical and spatial complementarity of SMIP binding sites toward the template, while the affinity for the analogue is very low. It is considered that the selective interaction between the polymeric matrices and template is ascribable to fluorine atom that takes an active part in interaction with the functional monomer.
Finally, the selectivity of the synthesised polymeric nanospheres can be highlighted by introducing another coefficient (ε) which is a quantitative measure of the imparted selectivity within the imprinted nanospheres and was calculated as the ratio between the amount (%) of 5-FU and U bound by SMIP. This value was found to be 2.3 in both organic and water media, indicating that imprinted polymers had higher affinity (more than 2 times) for 5-FU comparing to U.
As reported, hydrogels possess a degree of flexibility very similar to natural tissue, but in MIPs structure a compromise between the rigidity and flexibility of the polymers is needed. The structure of the imprinted cavities in the MIPs should be stable enough to maintain the conformation in the absence of the template and it should also be flexible enough to facilitate the attainment of a fast equilibrium between the release and re-uptake of the template in the cavity. In order to test swelling properties of the imprinted hydrogels, aliquots of nanospheres were immersed in swelling media: phosphate buffer at pH 7.4, simulating biological fluids. It can be observed from Figure 2.3 that the amount of water uptake by imprinted nanospheres increases with time and the maximum water uptake is obtained after 24 h (Table 2.2). These high swelling characteristics make the imprinted cavities of polymeric network easily accessible to the template; this is to advantage of recognition properties of imprinted nanospheres.
Figure 2.3 Swelling rate profile of SMIP.
3.3 In vitro release studies
After evaluation of imprinting effect of synthesised materials, their application as devices for 5-FU delivery in plasma simulating fluids was verified.
Different strategies were applied to determine the possibility to successfully employ an imprinted polymer to obtain a sustained/controlled release of the selected drug26.
In a first approach27, the loading step is performed by binding
experiments. After the incubation time, the supernatant is removed and the samples dried. In this way, different amounts of drug are bound by SMIP and SNIP according to the imprinting effect. In these conditions, because the releasing profile strongly depends on the loaded drug, SMIP particles are able to release a higher amount of drug than SNIP ones.
In another approach, more useful to emphasise the differences in the releasing profiles from SMIP and SNIP, both the polymers are loaded with the same amount of drug by mixing them with a drug standard solution. After the incubation time, samples were dried and release experiments performed. The
26 Alvarez-Lorenzo, C.; Concheiro, A. J. Chromatogr. B 2004, 804, 231. 27 Singh, B.; Chauhan, N. J. Macromol. Sci. A Pure Appl. Chem. 2008, 45, 776.
32 percentage of 5-FU released was calculated considering 100% the 5-FU content in dried samples28.
In our work, the second approach is employed and the presence of imprinted cavities in spherical polymers makes the release of the template more extended over time in comparison with non-imprinted materials. As it is possible to observe in Figure 2.4, indeed, while the drug is completely released within five hours by SNIP, that do not have specific binding cavities, for SMIP samples even after 50 hours the release is not yet complete. Such behaviour is in accordance with results obtained from the binding experiments.
Moreover, monodispersed spherical particles allow to obtain isotropic release behaviour and so also a better control of 5-FU release profile in comparison with materials with irregular size and shape.
Figure 2.4 5-FU release profile from SMIP ( ) and SNIP ( ) in plasma simulating fluids.
In order to further evaluate selectivity of SMIP, uracil release experiments in the same conditions tested with 5-FU were also performed. The data obtained from these experiments confirme the results showed in binding tests: uracil release from imprinted polymers, indeed, that just in 2 hours was
28 Pitarresi, G.; Pierro, P.; Giammona, G.; Iemma, F.; Muzzalupo, R.; Picci, N. Biomaterials 2004, 25, 4333.
33 completed, was remarkably faster than that obtained when 5-FU was used (data not shown).
In this work, 5-FU imprinted nanospheres with swelling characteristics were prepared using methacrylic acid and ethylene glycol dimethacrylate as functional monomer and crosslinker, respectively.
One-pot precipitation polymerisation, as synthetic technique to obtain the monodispersed particles, was chosen. The recognition properties and selectivity of synthesised materials were demonstrated through binding experiments with template and its analogue, uracil.
The results obtained from the in vitro release studies in plasma simulating fluids indicated that these polymeric matrices are also suitable for a controlled/sustained delivery of the tested anticancer agent in biological fluids. Hydrogel characteristic of these materials contributes to make binding sites in the polymeric network easily accessible to the template, while spherical shape allows to obtain a better control on 5-FU release.
Molecularly Imprinted Polymers for Selective Extraction and Sustained
Release of Glycyrrhizic Acid
Glycirrhiza glabra (liquorice) roots are extensively used in herbal medicines for their emollient, antitussive, anti-inflammatory, antiviral and gastroprotective properties1,2.
The product called “liquorice” in confectionery manufacturing (i.e. flakes or pastilles of pure liquorice) is obtained by treating dried G. glabra roots with boiling water, which is then evaporated to obtain a semi-solid extract3.
The main active compound of G. glabra is glycyrrhizin or glycyrrhizic acid (GL), also known as (3β, 20β) - 20 - Carboxy - 11 - Oxo - 30 - Norlean - 12 - En-3-yl-2-O-β-17- Glucopyranuronosyl- α- D-Glucopyranosiduronic acid. This molecule is present in the root and consists of an aglycon (a pentacyclic triterpenic structure) bound to two glucuronic acid molecules4. GL has been
demonstrated to possess anti-inflammatory, antiallergenic, antihepatotoxic, antiulcer and antiviral properties5,6 and is currently suggested as a possible
chemopreventive drug7. Furthermore, GL is one of the leading natural
compounds for clinical trials in recent studies on chronic viral hepatitis and
human immunodeficiency virus (HIV) infections8. Chronic consumption of GL
1 Sabbioni, C.; Ferranti, A.; Bugamelli, F.; Cantelli Forte, G.; Raggi, M.A. Phytochem. Analysis 2006, 17, 25.
2 Chung, J.G.; Chang, H.L.; Lin, W.C.; Wang, H.H.; Yeh, C.C.; Hung, C.F.; Li, Y.C. Food Chem. Toxicol. 2000, 38, 163.
3 Fenwick, G.R.; Lutomski, J.; Nieman, C. Food Chem. 1990, 38, 119. 4 Andersen, F.A. Int. J. Toxicol. 2007, 26, 79.
5 Ploeger, B.A.; Meulenbelt, J.; DeJongh, J. Toxicol. Appl. Pharm. 2000, 162, 177. 6 Aly, A.M.; Al-Alousi, L.; Salem, H.A. AAPS Pharm. Sci. Tech. 2005, 6, 74.
7 Ploeger, B.A.; Meulenbelt, J.; DeJongh, J. Toxicol. Appl. Pharmacol. 2000, 162, 177. 8 Arase, Y.; Ikeda, K.; Murashima, N.; Chayama, K.; Tsubota, A.; Koida, I.; Suzuki, Y.; Saitoh, S.; Kobayashi, M.; Kumada, H. Cancer 1997, 79, 1494.
36 prevents the development of hepatic carcinoma from C hepatitis and the antiviral activity of GL against SARS associated corona virus has been demonstrated in
vitro9. Finally, GL finds application in inhibiting unwanted effects of
contraceptive formulations, such as alterations in blood coagulation and thrombosis10.
Based on these considerations, the determination, the selective extraction of GL from liquorice roots and the development of a Drug Delivery System (DDS) for this compound have gained great interest.
Several papers report on analytical methods for the determination of GL with different techniques such as HPLC, capillary electrophoresis, gas chromatography, and high-performance thin layer chromatography11,12. In all
these techniques, different kind of sample preparation methods is required: plant extracts are, indeed, complex mixtures with a large variety of chemical compounds.
Among the extraction technique, Solid-Phase Extraction based on Molecularly Imprinted Polymers (MISPE) is an efficient approach for purification of analytes from complex matrices and preconcentration of the samples, and it is gaining considerable interest in environmental, clinical, and food analysis13,14,15.
Moreover, in recent years several studies are focused on the development of drug delivery systems based on polymeric materials and the importance of this research field is growing as ever more complex drugs and
9 Nassiri-Asl, M.; Hosseinzadeh, H. Phytoter. Res. 2008, 22, 709.
10 Stähli, B.E.; Breitenstein, A.; Akhmedov, A.; Camici, G.G.; Shojaati, K.; Bogdanov, N.; Steffel, J.; Ringli, D.; Lüscher, T.F.; Tanner, F.C. Arteriosclerosis, Thrombosis, and Vascular Biology 2007, 27, 2769.
11 Sabbioni, C.; Mandrioli, R.; Ferranti, A.; Bugamelli, F.; Saracino, M.A.; Cantelli Forti, G.; Fanali, S.; Raggi, M.A. J. Chromatogr. A 2005, 1081, 65.
12 Ohtakea, N.; Nakaib, Y.; Yamamotoa, M.; Sakakibarab, I.; Takedaa, S.; Amagayab, S.; Aburadac, M. J. Chromatogr. B 2004, 812, 135.
13 Anderson, R.A.; Ariffin, M.M.; Cormack, P.A.G.; Miller, E.I. Forensic Sci. Int. 2008, 174, 40.
14 Zhang, H.; Ye, L.; Mosbach, K. J. Mol. Recognit. 2006, 19, 248.
15 Benito-Peña, E.; Urraca, J.L.; Sellergren, B.; Moreno-Bondi, M.C. J. Chromatogr. A 2008, 1208, 62.
37 biopharmaceuticals are being developed, many of which cannot be administered without a controlled dosage system.
A controlled drug delivery system offers the possibility to maximise the drug efficacy and safety and to provide a suitable rate of delivery of the therapeutic dose, at the most appropriate site in the body, in order to prolong the duration of the pharmacological activity, to reduce the side effects and to minimise the administration frequency thus enhancing patient compliance16.
Among the different kind of polymeric materials applied in this research fields17 (erodible devices, implants, etc.), a particular attention have been
devoted to molecularly imprinted polymers (MIPs)18.
In this study, glycyrrhizic acid imprinted polymers were synthesised by the non-covalent imprinting approach, and a screening of the functional monomers (acidic, neutral or basic) was performed. After the evaluation of the imprinting efficiency, the best materials were tested as stationary phase in a SPE protocol for the selective extraction of GL from liquorice roots19 and as releasing
device20 in gastrointestinal simulating fluids.
2. Materials and methods
Ethylene glycol dimethacrylate (EGDMA), methacrylic acid (MAA), 2-(dimethylamino)ethyl methacrilate (DMAEMA), 2-hydroxyethyl metacrylate (HEMA), 2,2’-azoisobutyronitrile (AIBN), glycyrrhizic acid (GL) and glycyrrhetic acid (GA) were obtained from Sigma-Aldrich (Sigma Chemical Co., St. Louis, MO).
16 Cunliffe, D.; Kirby, A.; Alexander, C. Adv. Drug Deliv. Rev. 2005, 57, 1836. 17 Langer, R.; Peppas, N.A. AIChE J. 2003, 49, 2990.
18 Caro, E.; Marce, R.M.; Cormack, P.A.G.; Sherrington, D.C.; Borrull, F. J. Sep. Sci. 2006, 29, 1230.
19 Cirillo, G.; Curcio, M.; Parisi, O.I.; Puoci, F.; Iemma, F.; Spizzirri, U.G.; Restuccia, D.; Picci, N. Food Chem. 2011, 125, 1058.
20 Cirillo, G.; Parisi, O.I.; Curcio, M.; Puoci, F.; Iemma, F.; Spizzirri, U.G.; Picci, N. J. Pharm. Pharmacol. 2010, 62, 577.